261 49 4MB
English Pages 115
223 47 3MB Read more
256 38 2MB Read more
261 58 7MB Read more
Content: Role of C₄ hydrocarbons in aromatic species formation in aliphatic flames / J.A. Cole, J.D. Bittner, J.P. Longw
523 24 4MB Read more
296 15 32MB Read more
The discovery of high-temperature superconductivity  by Bendnorz and Muller in the La-BA-Cu-O system resulted in v
275 98 12MB Read more
FACTORS UNDERLYING!- THE COMBUSTION AT HIGH TEMPERATURES
SUBMITTED TO THE UNIVERSITY OF GLASGOW
FOR THE DECREE OF DOCTOR OF PHILOSOPHY
PATRICK TERENCE ARTHUR
ProQuest Number: 13870189
All rights reserved INFORMATION TO ALL USERS The quality of this reproduction is d e p e n d e n t upon the quality of the copy subm itted. In the unlikely e v e n t that the a u thor did not send a c o m p le te m anuscript and there are missing pages, these will be noted. Also, if m aterial had to be rem oved, a n o te will ind ica te the deletion.
uest ProQuest 13870189 Published by ProQuest LLC(2019). C opyright of the Dissertation is held by the Author. All rights reserved. This work is protected against unauthorized copying under Title 17, United States C o d e M icroform Edition © ProQuest LLC. ProQuest LLC. 789 East Eisenhower Parkway P.O. Box 1346 Ann Arbor, Ml 4 8 1 0 6 - 1346
CONTENTS page CHAPTER 1.
The Nature of Graphite and Amorphous C a r b o n
CHAPTER 11. The Mechanism of Carbon Combustion........
CHAPTER 111. Rie Combustibility Apparatus
CHAPTER IV. Combustion Under Varying Conditions of Gas Plow .20
The Effect of Temperature on Rate of Combustion .58
SUMMARY AND CONCLUSIONS.................................... 79
THE NATURE OF GRAPHITE AND AMORPHOUS CARBON
Before considering the combustion of carbon it is desirable to know something of the molecular nature of the material with which we are dealing*
It is usual to classify the various forms of carbon
as having either a diamond, graphite or an amorphous type of structure and it is with the two latter forms that we shall deal here.
The structure of graphite has been established by X-ray and chemical methods and itiis shown to consist of flat hexagon planes with a carboncarbon bond distance of 1.42 3.35
the distance between the planes being
Roth suggested, from data on heat of combustion, that
there were at least two different forms of graphite, termed "ex” and rt/3n, but this was not substantiated by the more accurate determinations of later workers-*-.
Since then, Lipson and Stokes^ have shown that X-ray
diffraction films indicate the existence of a modification of graphite in which the hexagonal layers are arranged with the fourth vertically over the first (the third layer is vertically over the first in the more usual structure) and this new form may be present to the extent of about 10 per cent, in natural graphite.
Ruff has suggested that the differences
in energy content and density between different samples of graphite may be due to the presence of faults in the graphite lattice.
Although there are powerful forces between the atoms of the layer planes of graphite, the inter-planar bond is extremely weak; it is 3 estimated by Ruff to be about one sixth of the strength of the bond between neighbouring carbon atoms in the same plane, whilst Pauling,
Fig. 1.- The structure of graphite.
\c / rC
Fig. 2.- One third double bond character of carbon atom in the graphite lattice.
Brockway and Beach
tend to neglect it altogether when they assume
that each bond has a one third double bond character corresponding to resonance among such structures as Fig. 2.
The high thermal and
electrical conductivity of graphite, comparable to that of many metals, suggests that the inter-planar bond may be regarded as a weak one dimensional metallic valency, and chemical evidence leads us to regard the graphite layer-planes as large free radicles bonded by weak valency forces to form graphite crystallites,
summarized in detail the similarity of the chemistry of graphite to that of the triarylmethyls.
It is evident from Fig. 3 that if we
consider one particular carbon atom in the graphite lattice then its three valency bonds lead to three aromatic hexagons and its proper ties might be expected to be similiar to those of the central carbon atom of the triphenylmethyl group.
The evidence accumulated leaves
little doubt as to the pronounced aromatic character of the hexagon layer-planes in pure graphite.
Our views on the structure of the so-called amorphous carbons have been considerably modified over the last few years.
as 1874 Weber® stated that the specific heats gave no evidence of three intrinsically different forms of carbon and this was confirmed by Debye and Scherrer^ who showed that the X-ray spectra of both graphite carbon and amorphous/vindicated the same internal crystal structure. There is abundant chemical evidence to support these views.
and amorphous carbon, e.g., soot, can form layered lattice structures such as
C^gK, (CF)n , etc., whilst Juetter^ has shown that the
yields of mellitic acid,
, a derivative of benzene, obtained
from carbonaceous materials heated to 1000 C. are of the same order
as those obtained from graphite*
The fact that the specific gravity
of the solid products of carbonisation is of the order of 1.9 as compared with the value of 2.25 for pure graphite is explained by the fact that, like most forms of commercial carbon, small quantities of gas (hydrogen, carbon monoxide*) are present between the graphite planes, thus preventing their coalescence and subsequent increase in density^* 16*
Blayden, Gibson and Riley-**1 have carried out extensive work on coals , cokes and chars by means of the X-ray powder diffraction tech nique applied to series of closely related specimens. coals and order.
c o k e s 1 *2
They suggest that
consist of platelets arranged in considerable dis
Bach platelet consists of several hexagon layer planes, -whose
edge atoms are linked to the non-carbon atoms present, and it is this -which limits the growth of the platelet.
By measuring the breadth
of the diffraction lines on the X-ray powder photograph it is possible to obtain a figure which is called the average crystallite dimension and it is found that, in general, these carbon crystallites contain three or four layer planes.
The latter, although parallel in any
one crystallite are arranged in randomly orientated groups and this type of structure has been termed by Warren1^ "turbostratic”.
ease with which the flat lamellae can move over one another appears to be decided by the presence of cross linkages (possibly through the agency of oxygen) and the terms rigid and mobile turbostratic systems have been coined.
More recently1^ tilting of the aromatic
hexagon planes similiar to thai^Liscussed by Karle and Brockway1*-* for the structure of o-tetraphenylene and analogous to that for glass1 6 has been put forward as a possible factor in the building
Pig. 3.- Similarity between a carbon atom in a graphite plane and in triphenyIme thy1 chloride.
up of cokes and chars*
As far as coal and coke are concerned we may agree with B o n e ^ and say that there is a gradual transition of benzenoid properties as the degree of coalification or carbonization proceeds.
nature of the original substance and the presence of foreign atoms are both of paramount importance, and the higher the temperature of carbonization the more likely is the material to approximate to an ordered graphite lattice.
Apart from considerations of internal molecular structure, combustion is also related to the macro structure of the burning particle.
It will be shown later that the rate of combustion of a
particle is directly proportional to its superficial surface area. The ratio of true to superficial surface is difficult to determine in the case of a porous char or coke but it appears from preliminary calculations, that for a material of a given porosity, it will be little affected bjr pore size and distribution.
Work is at present
being carried out on the relationship of the two latter factors to combustibility in the case of blast furnace coke.*
* Work at present in progress at the Royal Technical College, Glasgow.
THE MECHANISM OP CARBON COMBUSTION
Much work has been carried out on the carbon plus oxygen reaction both from a fundamental and an empirical point of view.
In order to
study the true surface reaction and avoid secondary reactions in the gas phase, it is necessary to conduct experiments at very low pressures, high gas velocities and with smooth carbon surfaces.
Work of this kind
has been carried out by Langmuir^, Sihvonen^and Meyer^, using electrically heated graphite filaments.
In some cases and attempt has
been made to correlate the results with the known structure of the graphite lattice (Sihvonen Constable
3v , Ruff ).
More recently, Strickland
has carried out low pressure experiments in a stationary
atmosphere, and he suggests convincingly that the conflicting results of earlier workers in this field may have been due to the activation of gas molecules by thermionic emission from the electrically heated filaments.
The results of this low pressure work cannot be extrapolated
to provide information on the combustion mechanism at higher pressures because of the complex diffusion problems and the presence of secondary gas phase reactions in the latter case.
Moreover, in the case of the
mechanism in beds of carbon particles, there is the additional complication of reactions within the voids of the bed.
Rhead and Wheeler
must be given the credit for the first
thorough investigation of the primary reaction between carbon and oxygen.
They put forward the conception of a surface complex CxOy
which then decomposed to give CO and OOg.
Similiar theories have since
been put forward by Lowry and Hulett^Rideal and Wright^, Shah27, and several other workers.
However , it has been pointed out
that the formation of a complex such as
that suggested by Rhead and Wheeler would lead to a zero order reaction since the rate of formation of the complex is high and its rate of decomposition is low, whereas Lambert2® , Meyer®®, and StricklandConstable2^ find the low temperature reaction (below 1500° JL) to be of the first order*
In addition, if surface compounds are formed
as above, the rate of reaction of freshly outgassed charcoal should increase as oxidation proceeds because initially oxygen will be used up to form a layer of surface oxide and only at a later stage will this decompose to give carbon monoxide and carbon dioxide*
contrary is found to be the case for the analogous reaction of charcoal with nitrous oxide*-*®.
Strickland-Constable puts forward the hypothesis
of two types of surface compound.
One of these, an "intermediate"
compound, is capable of oxidising carbon monoxide to carbon dioxide. He suggests that surface oxides are probably covalent compounds having a wide range of structure&nd thermal stability. borne out by Lowry and Hulett least 1000 charcoal.
who found that temperatures of at
C. were requiredto decompose all the solid oxides on
That these oxides may also, in certain cases, possess
distinct acid and basic properties has been shown by Schilow, Schatanowskaj a and Tschmutov
Strickland-Constable assumes pro
visionally that the intermediate compounds are the least stable of the surface oxides (or merely adsorbed oxygen) and that they react with more oxygen or carbon monoxide in the gas phase to form carbon dioxide by means of a first order reaction.
Work on active forms of carbon indicates that oxygen may be able to penetrate the hexagon layer planes of a graphite structure
to foim inter-planar oxides^.
However, it should be remembered
that the characteristic property of active carbon is its high specific surface reactivity which is due in part to an exceptionally large sur face area and inter-planar oxide formation may be of less importance for a non-reactive carbon*
When considering the mechanism of Hie oxidation reaction at higher pressures the number of intermolecular collisions in the gas phase becomes of supreme importance*
Several attempts have been made
to calculate absolute reaction rates of combustion on the assumption that the rate of diffusion of oxygen molecules towards the burning surface must balance the rate of diffusion of combustion products away from the surface.
Such methods are hampered by lack of detailed
knowledge concerning the physical conditions existing in the combustion zone.
Parker and Hottel
studied the gas film structure by micro
sampling of the adhering film and they calculated the diffusivities of carbon dioxide through nitrogen and oxygen through nitrogen.
workers assume a film of stagnant gas to surround the burning specimen when the problem of gaseous diffusion in considerably simplified. k
3 4 .
Burjte and Schumann
have applied this technique to the combustion of
small particles (less than 0.5 mm. diameter) of pulverized fuel. Smith and Gudmundsen^ describe experiments with carbon spheres of 4.6 mm. diameter, these being burnt in a stream of preheated air, and Mayers®® has set up an empirical equation based on their results to correlate the rate of combustion with variations in temperature, pressure, gas velocity and particle radius.
Tu, Davis, and Hottel
studied the rate of combustion of carbon spheres of 25 mm. diameter in dry preheated oxygen-nitrogen mixture^.
The sphere was suspended in
such a way that it was able to rotate at a standardized rate of 20 r.p.m.
As in the work of Smith and Gudraundsen the temperature of
the burning specimen was measured by means of an optical pyrometer. Tu, Davis and Hottel divided the process of combustion into two zones below about 1000° C. (surface temperature of the carbon), the rate of chemical reaction was said to control the rate of combustion and tem perature was all important whereas above
. diffusion was
suggested as the controlling factor and gas velocity became of greater importance.
Using the Reynolds analogy of fluid flow these Workers
were able to calculate approximately the absolute magnitude of the rate of combustion although they state that this analogy tends to predict unduly thin gas films when applied to such problems.
It may be noted
38 here that the use of Rice’s formula by Burke and Schumann for the calculation of the stagnant gas film thickness has been queried by Mayers
39 4-0 on the grounds of work by Kennard and by Page and Townend
neither Of wham obtained evidence of stationary films during their work on gas and liquid flow problems.
However, since Kennard was
dealing with the problem of temperature distribution surrounding bodies at temperatures of less than 150° C*, and Page and Townend were work ing on the flow of water in tubes at roam temperatures, it seems unwise to apply the conclusions of these comparatively low temperature experiments to the high temperature combustion process.
the existence of a stagnant film seems unlikely when one views the reaction on a coke surface by means of a high temperature microscope, the products of combustion being seen to disturb the fused ash at high temperatures.
On the other hand the existence of such a film
proved fruitful for purposes of calculation and indeed the remarkable 1
adherence of so£id ash to burning coke (p. 19 ) seems to justify such
an assumption in some cases*
Mayers4"*" in same experiments on the rate of reduction of carbon dioxide by graphite, passed carbon dioxide over cylindrical specimens of electrode graphite and by increasing the gas flow rate until no further increase in the rate of reaction was observed he was able to assume that at this flow rate the partial pressure of carbon dioxide at the surface of the specimen was equal to the total pressure of gas, i*e*, the velocity coefficient of partial pressure of carbon dioxide was zero.
In his subsequent calculations only those values of zero
velocity coefficient were used.
This method might be used for the com
bustion of carbon in oxygen but it would entail very high reaction rates which would be difficult to follow experimentally.
Finniston4 2 in a study of the combustion of coke used cylindrical specimens and burnt them in a stream of air at temperatures up to about 1500° C.
He was able to show that the rate of combustion was directly
proportional to the superficial surface area of the specimen and also to establish the validity of the Arrhenius conception of activation energy as applied to the combustion of coke.
Reference will be made
to this work later as it formed the starting point of the present research.
In conclusion, numerous empirical combustion tests have been designed for carbonaceous fuel beds, particularly coke, and
that physical conditions of sizing and voidage, etc., are of more im portance than the specific reaction rate of the fuel substance.
subject has beer^iscussed in some detail by Mayers4 3 and by Hiles and Mott
, the latter giving a summary of the Russian work in this field.
Plate 1.- Method of trepanning cylindrical coke specimens.
THE COMBUSTIBILITY APPARATUS As mentioned in the previous chapter it was decided to conduct further experiments along the lines of those carried out hy An H.M. Finniston
hut with some means of varying the factors of gas
velocity and pressure.
It was felt, moreover, that the effect of the
geometrical configuration of the combustion chamber in relation to the rate of combustion should be studied in some detail, as such variables as gas velocity and chamber diameter are mutually inter dependent.
The information from such geometrical considerations might
also be of value when studying the effect of voidage and packing density in a fuel bed.
Although this work applies to the combustion of carbon in general# its application to the combustion of coke in the blast furnace for the production of pig iron has been kept constantly in view.
reason most of the work has been carried out on specimens of coke* these being either cut from large pieces with a diamond cutting wheel and ground to shape or drilled out by means of a diamond tipped trepanning tool as shown in Plate 1.
In the formepfease each specimen
in the form of a cylinder measured 3.18 cm. long and 1.91 cm. diameter, whereas in the latter case the diameter was 1.83 cm.
method is much to be preferred both from the point of view of accuracy of shape and also labour involved, but the method is not suitable for badly fissured coke.
The essential requirement is a high speed drill
of extreme rigidity with provision for the application of ample water to the grinding surfaces.
All specimens were finally drilled axially
with a e i*1* (°* 32 on*) high speed steel drill for the purpose of suspension*
As far as possible the coke specimens were free
cracks and they were cut from the centre of half-oven width pieces, i* e*, the soft centre—oven ends and the badly fissured cauliflower endsj/fcrere neglected*
By this means it was possible to obtain specimens
of approximately constant density from the same sample of coke, the weight remaining constant to within ±0 .3 gm., the total weight of the specimen varying from 7 to 9 gm* according to the coke used.
Each specimen was suspended from a silica tube to which was fused a small platinum hook and this was then attached to a nichrome wire.
The loss in weight of the suspension during a run, from reduc
tion of the silica, was less than
0 .0 1
gm. and could be neglected.
At temperatures above 1550° G. the silica suspension wa^ound to have insufficient strength to support the specimen and it was replaced by a fused alumina tube.
The gas for the combustion was drawn through the apparatus by means of vacuum pumps A and B (Fig. 4), the former being an Edwards Speedivac 1A with a rated capacity of 48 litres per minute, and the latter an# Edwards Hyvac of 10 litres per minute capacity, this being used mainly as a standby when an extra large capacity was required and also for the purpose of calibrating the gas flow as described below.
It was feared at first that the products of combustion contain
ing sulphur dioxide (obtained from the oxidation of sulphur in the coke) might corrode the working parts of the pumps, but they functioned perfectly satisfactoredty and no material damage appears to have been sustained over a period of some two and a half years, the vacuum oil being renewed about every six months.
«* Fig. 4.- Gas flow diagram for the combustion apparatus.
When using air for combustion it was dried "by drawing it through concentrated sulphuric acid and then through a tower packed with alternate layers of magnesium perchlorate and glass wool in Train (l)of Pig* 4.
In order to study the effect of varying oxygen concentra
tion, a second train (2 ) was added, and this could he supplied with either pure oxygen or pure nitrogen from cylinders of the compressed gas.
Taps d and d* were used to regulate the flow of gas required and
once these had "been correctly adjusted for a particular rate of gas flow c and c* were used for ”ontt and "off" regulation only.
and b* were left open tod the gas cylinder valves adjusted to provide a slight excess of gas over that actually required, the excess being blown off to atmosphere, and in this way a constant pressure head h was maintained. an
Prom the drying towers the gases were passed to
litre bottle S, thence through tap g to the combustion chambe^.
Owing to the fact that in same cases gas was being supplied from a cylinder at a pressure greater than atmospheric, whilst in other cases air was being drawn from the atmosphere, the conventional forms of gas metering apparatus were not found to tbe^ tinuous range of gas flow from about required.
Moreover, a con
to 8000 ml. per minute was
For this reason the following method of gas measurement
was devised and it was found to be ideally suited to the desired requirements. Suppose bottle S is exhausted until the pressure of gas in it is p, the volume of gas in S (at N.T.P.) is then given by Vq = kp
where k is a constant.
Now allow gas to flow into S for a time dt, Then the pressure will rise to a value (p + dp) and the volume of gas will then be given by V 2 = k(p + dp)
Hence the rate of gas flow over the time dt is given by
If “ bottle S is evacuated/and gas then allowed to flow through tap d and measurements made of pressure and time it is found, as shown in Fig. 5 for a wide range of gas flow rates, that dp/dt is constant as long as p is less than about 40 cm. of mercury pressure, i.e., for a given setting of tap d, the ga^flows at a constant rate into bottle S provided that the pressure in S never rises above 40 cm. of mercury.
It is difficult to show why this should be so from
a theoretical point of view as the problem of gas flow through a short tube (corresponding to tap d) with a large pressure drop across the ends is an exceedingly complex one and most mathematical treatments 4.c
neglect turbulence and deal with gases at very low pressures
If S is exhaustedto a pressure p^ the volume of gas it contains at N.T.P. is given by Vi = V 3 .2 p.P- 1 / 7 6
where V s is the volume of bottle S and T the gas temperature in p^ is measured in cm. of mercury.
Suppose gas is now allowed to flow
through tap d into S until a pressure of pj + 20 is reached (an increase in pressure of
cm. was found to be the most convenient for purposes
of gas flow calibration), then the volume of the gas in S at N.T.P. is ^2 =
(pi + 20)/76
i.e. the change of volume is
v 2 - Vi = V
c e n t im e t r e s
T i m e - Se c o n d s .
.- Results illustrating the constancy of dp/dt for the gas flow measurement apparatus.
The figures on the curves
refer to rates of gas flow in ml. per minute.
If the time taken for this 20 cm. rise of pressure is t seconds then, since dp/dt is a constant (for p less than 40 cm.) we may say that the rate of flow is V r .273.20 I.76.t ml/sec. t V s can he obtained by filling the bottle S with water and weighing, and hence we may express the rate of flow as K»1 T t
ml. per second.
where K is a constant which can be readily calculated.
By varying the opening of tap d a chart was constructed of rate of gas flow plotted against "the time for an increase in pressure of 20 cm. of mercury, the room temperature T being taken as 295° A.
small correction was easily made for room temperature variation when reading from this chart and it wa^found that variations in atmospheric pressure had a negligible effect .
The accuracy of this method of
gas flow measurement was always within +1.5 per cent.
During an actual run, gas was drawn continuously through the apparatus, the pressure to the left of taps d and d* (Fig.4) being always less than 40 cm., whereas the pressure on the right hand side was always approximately 76 cm.
As there was a pressure drop of abodt
0.5 cm. from S to the combustion chamber, the manometer M was connected by taps f and k to either one or the other, according to which pressure was being measured ai^the time.
When checking the gas flow rate it
was found convenient to isolate the furnace chamber and use pump B for evacuating S.
The furnace used for these combustion experiments is shown in
i late 11* - General view of the combustibility apparatus*
and a general view of the combustion apparatus is shown in
The winding of the molybdenum wound electrical resistance
furnace was protected from oxidation by the passage of a continuous stream of cracked ammonia*
The latter was produced by passing gaseous
ammonia from a cylinder through red hot mullite tubes packed with mild steel turnings.
This decomposed the ammonia into its constituent
elements which were then passed successively through water, to remove any undecomposed ammonia, sulphuric acid to remove water vapour, and finally granulated zinc to remove any sulphuric acii spray.
combustion chamber itself consisted of a mullite tube (Morgan*s Triangle H5 quality) of about 5 cm. internal diameter and it was water cooled at both ends to prevent overheating and burning of the rubber bungs*
The gas for combustion was introduced at the bottom
and preheated in its passage through three alumina baffle plates drilled with fine holes, these plates being attached to a 9 mm* external diameter closed end mullite tube containing a calibrated platinum/13 per cent, platinum-rhodium thermocouple.
In some pre
liminary experiments with an open ended thermocouple sheath, gas was drawn in-to the furnace over the baffle plates and then back through the sheath and so out of the furnace.
In this way the preheated gas
was drawn over the bare end of the thermocouple and the results suggested that the gas was actually preheated to the temperature of the
combustion ehamber. The distance
between the top of the thermo
couple and the bottom of the burning specimen was 1.0 cm.
taken to wind the furnace in such a way as t6 produce a uniform
zone over a length 6
length being about
about 7 cm.,the maximum
variation along this
° C. while the temperature variation across a
diameter of the furnace tube was less than 3